**Vibrational Properties of Hexagonal Boron Nitride: Inelastic X-Ray Scattering**

**and Ab Initio Calculations**

**and Ab Initio Calculations**

J. Serrano,1,*A. Bosak,1R. Arenal,2M. Krisch,1K. Watanabe,3T. Taniguchi,3H. Kanda,3A. Rubio,4,5and L. Wirtz6,5
1_{European Synchrotron Radiation Facility, Boıˆte Postale 220, 38043 Grenoble, France}

2* _{Materials Sciences Division, Argonne National Laboratory, Argonne, Illinois 60439, USA}*
3

_{National Institute for Materials Science, 1-1 Namiki, Tsukuba, 305-0044, Japan}4_{Departamento de Fı´sica de Materiales, Facultad de Ciencias Quı´micas, Universidad del Paı´s Vasco, Centro Mixto CSIC-UPV/EHU}*and Donostia International Physics Center, E-20018 San Sebastia´n, Basque Country, Spain*

5* _{European Theoretical Spectroscopy Facility (ETSF), E-20018 San Sebastia´n, Basque Country, Spain}*
6

_{IEMN (CNRS-UMR 8520), Boıˆte Postale 60069, 59652 Villeneuve dAscq Cedex, France}(Received 14 December 2006; published 1 March 2007)

The phonon dispersion relations of bulk hexagonal boron nitride have been determined from inelastic
*x-ray scattering measurements and analyzed by ab initio calculations. Experimental data and calculations*
show an outstanding agreement and reconcile the controversies raised by recent experimental data
obtained by electron-energy loss spectroscopy and second-order Raman scattering.

DOI:10.1103/PhysRevLett.98.095503 PACS numbers: 63.20.Dj, 61.10.Eq, 63.10.+a, 71.15.Mb

Besides their intermediate structure between
two-dimensional sheets and 3D crystals, layered compounds
are relevant materials for storage of other compounds [1]
and as potential building blocks for nanotubes [2]. Among
these materials, graphite and hexagonal boron nitride
*(h-BN) have drawn most of the attention due to their*
simple hexagonal structure, their fascinating properties,
and the successful realization of carbon- [3] and more
recently BN [4–6] nanotubes. A wide band gap
*semicon-ductor, h-BN, has been grown successfully very recently as*
a single crystal. It exhibits a lasing behavior at 5.8 eV that
makes it attractive for optoelectronic applications in the
ultraviolet energy range [7].

Despite the tremendous effort devoted to the
*character-ization of physical properties of h-BN, the lattice *
dynam-ics, responsible for the elastic and thermodynamic
properties such as the heat capacity and the thermal
ex-pansion, are still under debate. First principles calculations
are generally accepted as the most accurate theoretical
description of the lattice dynamics [8]. Recently, for
*h-BN, the validity of state of the art ab initio calculations*
*was put in doubt by two experiments: Rokuta et al. [*9]
reported the only experimental data available for the
pho-non dispersion relations by electron-energy loss
*spectros-copy (EELS) performed on a monolayer of h-BN deposited*
on a Ni(111) substrate. Among several deviations from
*ab initio calculations of the lattice dynamics both for a*
monolayer [10,11*] and for bulk h-BN [*12,13], the EELS
*data show a degeneracy at the K point between acoustic*
*(ZA) and optical (ZO) modes polarized along the c axis.*
The origin of this degeneracy has not been clarified yet.
More recently [14], second-order Raman spectra of single
*crystalline h-BN revealed two features that contested the*
predictions based on a simple doubling of the energy scale
*of ab initio calculations for the one-phonon density of*
states, suggesting deviations up to 40% for the calculated

*energy of the TA branch in the K-M region. Since h-BN is*
a relevant material for UV lasing, it is imperative to resolve
the existing controversies and critically assess the quality
*of the ab initio calculations. Furthermore, we need exact*
information on the lattice dynamics in order to properly
understand the contributions due to electron-phonon
cou-pling observed in the cathodoluminescence and absorption
*spectra of h-BN [*7] and BN nanotubes [15,16].

In this Letter we address the above discrepancies in the
vibrational properties by reporting inelastic x-ray
scatter-ing (IXS) measurements and first principles calculations of
*the phonon dispersion relations of bulk h-BN. We also*
*report ab initio calculations of the phonon dispersion of a*
*monolayer of h-BN on a nickel substrate. Our results and*
analysis yield a complete picture of the lattice dynamics of
*h*-BN, reconcile theoretical and experimental data, and
reveal the origin of the controversies raised by the EELS
and Raman data.

Room temperature IXS measurements were conducted
on beam line ID28 at the European Synchrotron Radiation
*Facility in Grenoble using h-BN single crystalline flakes of*
*typical sizes of 500 200 50 m*3 _{with the surface}
*oriented perpendicular to the c axis. Monochromatic*
x rays of 17.794 and 15.817 keV were utilized to achieve
an energy resolution of 3 and 5.5 meV, respectively.
*Furthermore, ab initio calculations were performed for*
the phonon dispersion relations and the eigenvectors using
the ABINIT code [17,18], based on the linear response
method [19] and within the local density approximation
of density functional theory [20].

*With 4 atoms in the unit cell and space group P6*_{3}*=mmc,*
*h*-BN phonon dispersion relations show 12 branches that
*can be divided into the 2E1u 2A2u 2E2g 2B1g*
irre-ducible representations at the Brillouin zone center. The
*E _{1u}and A_{2u}are infrared active, the E_{2g}*are Raman active,

*and the out-of-plane polarized B*modes, also

_{1g}**denomi-PRL 98, 095503 (2007)**P H Y S I C A L R E V I E W L E T T E R S 2 MARCH 2007week ending

nated ZA and ZO modes, are silent. The acoustic modes
*have symmetry E _{1u} A_{2u}*and the crystal field gives rise to
a splitting between longitudinal (LO) and transverse

*opti-cal phonons for the other E1u*

*modes, whereas the E2g*modes remain doubly degenerate each. In Table I we compare our calculations with the experimental data re-ported for the point by Raman [14,21–24] and infrared [22,25] spectroscopy. The agreement between both data sets is excellent, the largest difference being a 5%

*under-estimate of the A*mode, similar to that reported by

_{2u}*previous ab initio calculations [*12,13

*]. The high E*

_{2g}mode, marginally overestimated, is related via zone
*fold-ing to the A*_{1} mode that dominates the Raman spectra of
BN nanotubes [11,26].

Figure1displays selected IXS spectra of the TA modes
*along the [110] (-K-M) direction, polarized along the*
*c*axis. The Stokes and anti-Stokes peaks are observed in
*the spectra taken at low momentum transfer q and a*
*decrease of the intensity with increasing q is apparent.*
This mode exhibits a paraboliclike energy dependence at
*low q, typical for layered materials, and flattens towards*
the edge of the Brillouin zone, in excellent agreement with
the calculated dispersion. The calculations predict the
*ob-servation of the ZA acoustic branch only for q q L *
*mo-mentum transfers with odd L, in agreement with the upper*
branch in the inset of Fig.1*obtained for L 3 and with*
the absence of these modes in the displayed spectra,
*cor-responding to momentum transfers with L 6. The IXS*
data for the acoustic phonons has been employed for the
determination of the five independent components of the
*elastic stiffness tensor of h-BN [*27], providing an upper
limit of 0.81 TPa for the axial elastic modulus of BN
single-wall nanotubes, in agreement with several theories
(0.85 TPa, [28,29] ) and recent electric-field induced
reso-nance experiments (0.722 TPa, [30] ).

Figure2(a)shows the experimental IXS phonon
*disper-sions compared with the ab initio calculations (solid lines).*
The solid (open) circles correspond to modes polarized
*mainly along the c axis (in-plane) and Raman and infrared*
data are shown as open (green) and solid (magenta)
dia-monds, respectively. We shall emphasize the excellent

TABLE I. Experimental and calculated phonon energies (in meV) at the point.

Symmetry Experiment Theory

*E2g* 6.4a 6.5
*B1g*ZA silent 15.0
*A2u* 97.1b 92.6
*B1g*ZO silent 100.4
*E2g* 169.4a, 169.9c, 169.1d 171.0
*E1u*TO 169.5b 170.9
*E1u*LO 199.6b 199.7
a_{Raman data [}_{21}_{].}
b_{Infrared data [}_{22}_{].}
c_{Raman data [}_{22}_{].}
d_{Raman data [}_{14}_{].}

FIG. 1 (color online). *Representative IXS spectra of h-BN for*
*the TA branch along the [110] direction, polarized along the c*
axis. The symbols represent the IXS data whereas the solid (red)
curves display the least-squares fit. The corresponding portion of
*the phonon dispersion is shown in the inset, where q is given in*
reciprocal lattice units (r.l.u.). The IXS data of the upper branch
*(ZA) were obtained for q q 3 total momentum transfers.*

Γ A 0 25 50 75 100 125 150 175 200 Energy [meV] ZA TA LA ZO TO LO LO M K Γ 0K Γ 25 50 75 100 125 150 175 200 ) b ( ) a ( HREELS

FIG. 2 (color online). *(a) Phonon dispersion relations of h-BN*
along the main symmetry directions. The open (red) circles
display modes polarized in the hexagonal plane whereas the
*solid (blue) circles correspond to modes polarized along the c*
axis. The solid curves represent the calculated phonon dispersion
and infrared [22] and Raman [14,21,22] data at the point are
displayed by open (magenta) and solid (green) diamonds.
*(b) Calculated phonon dispersions of a monolayer of h-BN*
deposited on 3 layers of Ni (solid lines) compared to the
EELS data from Ref. [9] (red open circles). Note that in the
experiment only vibrational modes involving boron or nitrogen
atoms were detected while in the calculations also the vibrational
modes of the Ni substrate are included.

**PRL 98, 095503 (2007)** P H Y S I C A L R E V I E W L E T T E R S 2 MARCH 2007week ending

agreement between the calculated and IXS dispersions.
Our calculations do not suffer from the negative energies
displayed in Ref. [13] and reproduce the energy of the
lowest lying Raman mode (shear mode) at 6.4 meV [21],
*improving upon those by Kern et al. [*12]. This may be due
to a combination of a larger energy cutoff for plane-wave
expansion of the wave functions and the use of slightly
larger lattice parameters [20]. Slight deviations occur for
the high energy TO modes and amount to less than 3%,
within the expected accuracy of this kind of calculations.
Previous theoretical data [12,13] did not provide an
accu-rate description of the quasiacoustic branches along the
*-A direction.*

The ZA-ZO splitting predicted by the theoretical models
*at the K point is well reproduced by the IXS data. Contrary*
*to this, in the EELS measurements of Rokuta et al. [*9] on a
*monolayer of h-BN deposited on a Ni(111) substrate, an*
*almost degeneracy of ZA and ZO was found at K. We*
investigated two reasons that might lead to this almost
*degeneracy: (i) charge transfer from the h-BN monolayer*
to or from the substrate and (ii) the influence of the
interlayer interaction with the substrate. As for the effect
of charge transfer, we calculated the phonons for a charged
*single sheet of h-BN. Negative charging leads indeed to a*
*closing of the gap between the ZA and ZO modes at K.*
However, a charging with 0.3 electrons per unit cell is
*necessary to reach degeneracy at K. This is in contrast to*
earlier calculations of the electronic structure of a single
*h*-BN sheet on nickel where a transfer of 0.06 electrons to
the substrate, i.e., a slightly positive charging of the sheet,
was predicted [31]. We therefore conclude that charge
transfer cannot be the origin of the degeneracy in the
*experiment of Rokuta et al. We performed an ab initio*
calculation of the phonon dispersion of a BN sheet on
nickel to investigate the influence of the interaction with
the substrate, simulated by three monolayers of Ni. The
calculated dispersion and the EELS data are in excellent
agreement, as displayed in Fig.2(b). The differences
be-tween the EELS and IXS dispersions can therefore be
*attributed to the bonding between the h-BN monolayer*
and the Ni substrate. Indeed, the calculations of Grad
*et al. [*31*] had revealed a strong hybridization of the *
*orbitals of BN with the d levels of nickel, a polarization of*
*the h-BN layer due to the substrate, and a substrate induced*
*exchange splitting of electrons in the band of h-BN. The*
*-d hybridization and a strong chemisorption have also*
been revealed by core electron and photoemission
spec-troscopies [32,33]. We can therefore conclude that the
observed softening of the ZO branch stems from the
bind-ing of the layer to the substrate.

Figure3reproduces the second-order Raman spectrum
*of h-BN reported by S. Reich et al. in [*14]. They compare
their results with calculations of the one-phonon density of
states (DOS) [12] for which the frequency scale has been
multiplied by 2. This comparison implicitly assumes that

the overtones, i.e., sums of modes with the same frequency,
are much stronger than combinations of phonons
belong-ing to different branches. Although most of the spectral
features are successfully assigned based on a detailed
group theoretical analysis and the above assumption, the
*peaks found at 114 and 284 meV (labeled B and H in*
Fig.3) were not compatible with the assignment. This led
the authors to conclude that the calculated frequencies are
too small to describe the spectra. The excellent agreement
between IXS data and our calculations is in stark
disagree-ment with this conclusion. The dotted (blue) line in Fig.3

corresponds to our calculated one-phonon DOS scaled in
the same way as the one used for comparison with the
Raman data in Ref. [14]. The dashed (red) line, however,
represents the full two-phonon DOS, taking into account
both overtones and combinations. A wealth of new spectral
features is obtained in this way and two of the strongest
ones lie underneath the experimental features under
dis-cussion. In view of this agreement between the two-phonon
DOS and the Raman spectra, we have analyzed the
assign-ments of the other features and the result is summarized in
TableII. Using the IXS data and the calculated dispersions,
*we therefore assign peaks B and H to combinations of*
*ZA ZO and LA LO modes at the K point. *
Further-more, the unknown peak reported at 2800 cm1
*(347.2 meV, labeled L) may be assigned to a combination*
*of LO and TO modes at the overbending along the -K and*
*-K-M directions. Beside these peaks, there is a general*
agreement with the assignments reported in [14], the
dis-crepancies stemming from the explicit consideration of
combination of modes with different frequency.

0 50 100 150 200 250 300 350 400

## Energy [meV]

## Raman Intensity

TO, LO (Γ) A B C DEF G H I J K LM NOFIG. 3 (color online). Comparison of the second-order Raman
*spectrum of h-BN (solid, black) reported in Ref. [*14] with our
calculations for the one-phonon (dotted, blue line) and
two-phonon (dashed, red line) DOS. The energy axis of the
one-phonon DOS has been multiplied by a factor 2, in the same
fashion as in Ref. [14]. The most relevant features of the
experimental spectrum are labeled, and their energies compared
with IXS data and calculations in TableII.

**PRL 98, 095503 (2007)** P H Y S I C A L R E V I E W L E T T E R S 2 MARCH 2007week ending

In summary, we have reported the phonon dispersion
*relations of bulk h-BN obtained by IXS and ab initio*
calculations. The IXS data are in excellent agreement
with the calculated dispersion and previously reported
Raman and infrared data. The discrepancies observed
be-tween EELS and IXS data stem from the polarization of the
*h*-BN monolayer due to the nickel substrate, a fact that
poses a challenge in measurements of elastic and optical
properties of BN nanotubes deposited on metallic
sub-strates. The alleged discrepancies between calculations
and second-order Raman spectral features disappear
when one takes into account phonon combinations by
calculating explicitly the two-phonon DOS.

We gratefully acknowledge F. J. Manjon, M. Muntwiller, and M. Hoesch for fruitful discussions. A. R. and L. W. acknowledge support by the European Community Network of Excellence Nanoquanta (No. NMP-CT-2004-500198). L. W. acknowledges funding by the French ANR and A. R. by the SANES project (No. NMP4-CT-2006-017310), Basque Country University, and MCyT. Calculations were performed at IDRIS and at the Barcelona Supercomputing Center.

*Electronic address: jserrano@esrf.fr

[1] M. S. Dresselhaus, G. Dresselhaus, K. Sugihara, I. L.
Spain, and H. A. Goldberg, *Graphite* *Fibers* *and*
*Filaments (Springer-Verlag, Berlin, 1988).*

**[2] J. Nagamatsu et al., Nature (London) 410, 63 (2001).**

**[3] S. Ijima, Nature (London) 354, 56 (1991).**
**[4] N. G. Chopra et al., Science 269, 966 (1995).****[5] R. S. Lee et al., Phys. Rev. B 64, 121405 (2001).****[6] R. Arenal et al., Phys. Rev. Lett. 95, 127601 (2005).****[7] K. Watanabe, T. Taniguchi, and H. Kanda, Nat. Mater. 3,**

404 (2004).

**[8] S. Baroni et al., Rev. Mod. Phys. 73, 515 (2001).****[9] E. Rokuta et al., Phys. Rev. Lett. 79, 4609 (1997).****[10] L. Wirtz et al., Phys. Rev. B 68, 045425 (2003).****[11] L. Wirtz et al., Phys. Rev. B 71, 241402(R) (2005).****[12] G. Kern, G. Kresse, and J. Hafner, Phys. Rev. B 59, 8551**

(1999).

**[13] W. J. Yu et al., Phys. Rev. B 67, 014108 (2003).*** [14] S. Reich et al., Phys. Rev. B 71, 205201 (2005).*
[15] B. Arnaud

*et*

*al.,*Phys. Rev. Lett.

**96,**026402

(2006).

**[16] L. Wirtz, A. Marini, and A. Rubio, Phys. Rev. Lett. 96,**
126104 (2006).

[17] TheABINIT code is a common project of the Universite´ Catholique de Louvain, Corning Incorporated, and other contributors (URL: http://www.abinit.org).

**[18] X. Gonze et al., Comput. Mater. Sci. 25, 478 (2002).****[19] X. Gonze and C. Lee, Phys. Rev. B 55, 10 355 (1997).**
[20] The wave functions of valence electrons were expanded in

plane waves with an energy cutoff of 40 a.u. Core
elec-trons were replaced by Troullier-Martins
pseudopoten-tials. A 9 9 4 sampling was used for the integration
over the Brillouin zone. Geometry optimization yielded an
in-plane lattice constant of 2.496 A˚ and an interlayer
distance of 3.254 A˚ . The dynamical matrix was calculated
*on a 14 14 6 q grid and interpolated in reciprocal*
space for the calculation of phonons at an arbitrary phonon
*wave vector q.*

[21] R. J. Nemanich, S. A. Solin, and R. M. Martin, Phys. Rev.
**B 23, 6348 (1981).**

**[22] R. Geick, C. H. Perry, and G. Rupprecht, Phys. Rev. 146,**
543 (1966).

**[23] T. Kuzuba et al., Phys. Rev. B 18, 4440 (1978).**

**[24] G. J. Exarhos and J. W. Schaaf, J. Appl. Phys. 69, 2543**
(1991).

**[25] P. J. Gielisse et al., Phys. Rev. 155, 1039 (1967).****[26] R. Arenal et al., Nano Lett. 6, 1812 (2006).**

**[27] A. Bosak et al., Phys. Rev. B 73, 041402(R) (2006).****[28] E. Hernandez, Phys. Rev. Lett. 80, 4502 (1998).**

[29] K. N. Kudin, G. E. Scuseria, and B. I. Yakobson, Phys.
**Rev. B 64, 235406 (2001).**

* [30] A. P. Suryavanshi et al., Appl. Phys. Lett. 84, 2527*
(2004).

* [31] G. B. Grad et al., Phys. Rev. B 68, 085404 (2003).*
[32] A. B. Preobrajenski, A. S. Vinogradov, and N. Martensson,

**Phys. Rev. B 70, 165404 (2004).**

[33] A. B. Preobrajenski, A. S. Vinogradov, and N. Martensson,
**Surf. Sci. 582, 21 (2005).**

TABLE II. Experimental and calculated energies (in meV) for relevant features of the second-order Raman spectrum.

Label (Fig.3)

Raman

[14] Assignment IXS Theory

A 76.9 *2ZAM* 78.8 78.8
B 114.1 *ZA ZOK* 115.2 111.9
C 203.3 2ZO 200.8
D 224.4 *ZO LAM* 221.5 221.2
E 233.1 *ZO TOK* 234.1 233.2
F 238.1 *TA LAK* 242.1 240.7
G 265.3 *TA LOK* 269.0 265.3
H 283.9 *LA LOK* 289.9 286.9
I 300.0 *LA TOM* 298.8 302.7
J 314.9 *2TOM-K* 317.8 320.5
K 338.5 *2TO; 2LO* 341.8
L 347.2 *LO TOoverb:* 346.8 347.7
M 364.5 2LO(overb.) 364.7 365.5
N 378.2 LO TO 374.3
O 398.0 2LO 399.4

**PRL 98, 095503 (2007)** P H Y S I C A L R E V I E W L E T T E R S 2 MARCH 2007week ending